EUTECTIC TRANSFORMATION IN DUCTILE CAST IRON. PART I THEORETICAL BACKGROUND


 Kellie Washington
 2 years ago
 Views:
Transcription
1 METALLURGY AND FOUNDRY ENGINEERING Vol. 31, 005, No. Edward Fraœ *, Marcin Górny **, Hugo F. López *** EUTECTIC TRANSFORMATION IN DUCTILE CAST IRON. PART I THEORETICAL BACKGROUND SYMBOLS Symbols Meaning Definition Units a Material mould ability to absorb of heat a = kmcm J/(cm ºC s 1/ ) A Parameter Eq. (10) s 1/ /m b Nucleation coefficient of graphite Eq. (58) o C B Temperature parameter Eq. (14) c Specific heat of metal Table 1 J/(cm 3 ºC) c m Specific heat of mould material J/(cm 3 ºC) C Carbon content in cast iron wt. % C e Carbon content in graphite eutectic Eq. () wt. % CT Chilling tendency Eqs. (67), (68) s 1/ / o C 1/3 C, C 3, C 4, C gr Carbon content in austenite, liquid and graphite Fig (3b) wt. % D Diffusivity of carbon in austenite Eq. (64) cm /s f gr Fraction of preeutectic graphite Eq. (1) * Prof., ** Ph.D., Faculty of Foundry Engineering, AGH University of Science and Technology, Cracow, Poland; ** Author is an award holder of the NATO Science Fellowship Programme *** Prof., Department of Materials Engineering, University of WisconsinMilwaukee, P.O. Box 784, Milwaukee, WI 5301, USA; 113
2 F c Surface area of the casting cm F ch Half surface area chill triangle Figure11 cm k Coefficient Eqs. (39), (43) k m Heat conductivity of the mould material J/(s cm ºC) l s l Size of substrate for nucleation of graphite Mean size of substrates for nucleation of graphite cm cm L e Latent heat of graphite eutectic Table 1 J/cm 3 m gr Mass of graphite Eq. (31) g m l Mass of graphite in liquid Eq. (30) g m γ Mass of graphite in austenite Eq. (35) g M Casting modulus Eqs. (11), (5), (55) cm M cr Critical casting modulus Eq. (70) cm N Volumetric nodule count Eqs. (57), (6) cm 3 N s Density of substrates for nucleation of graphite cm 3 P cr Coefficient Eq. (66) (cm o C 1/3 )/s 1/ P Phosphorus content in cast iron wt. % q a Accumulated heat flux in casting Eq. (6) J/s q m Heat flux extracted from casting into mould casting Eq. (5), (50) J/s q s Heat flux generated during solidification Eq. (7),(49) J/s Q Metal cooling rate Eq. (15) ºC/s R 1 Graphite nodule radius Figure 3b cm R Outer radius of austenite envelope Figure 3b cm R m Austenite envelope radius at maximum undercooling Eq. (47) cm s Wall thickness cm s cr Critical wall thickness Eqs. (71), (7) cm Si Silicon content in cast iron wt. % 114
3 t Time s t m Time at the maximum undercooling Eq. (1) s t s Time at the onset of graphite eutectic solidification s T Temperature ºC T c Equilibrium temperature of the cementite eutectic Table 1 ºC T i Initial temperature of metal in mould cavity ºC T m Temperature at maximum undercooling of graphite eutectic Figure a ºC T p Pouring temperature ºC T s Equilibrium temperature of the graphite eutectic Table 1 ºC V c Volume of casting cm 3 z Parameter Eq. (54) α Wedge angle Figure 11 o α d Thermal diffusivity of mould material k m /c m cm /s β Coefficient Table 1 o C 1 ΔH Enthalpy of metal J/cm 3 ΔΤ Undercooling of graphite eutectic ΔΤ m Maximum undercooling of graphite eutectic ΔΤ m = T s T m ºC ΔΤ sc Range of temperature, ΔΤ sc = T s T c Table 1 ºC θ Wetting angle between substrate and nuclei of graphite o ρ l Density of melt Table 1 g/cm 3 ρ gr Density of graphite Table 1 g/cm 3 ρ γ Density of austenite Table 1 g/cm 3 σ Interfacial energy between the nucleus and the melt J/cm ϕ, ϕ 1 Parameters Eqs. (5), (6) % ω Frequency Eq. (17) 1/s 115
4 1. INTRODUCTION Ductile cast iron is a modern engineering material whose production is continually increasing. Hence, there are numerous reports related to the production of nodular cast iron, some of which are of essential importance as they are linked to the solidification kinetics. In ductile cast iron, solidification is closely related to the nucleation and growth of nodular graphite. Yet, nucleation is the dominant process at the onset of solidification and it establishes the final nodule count. Accordingly, increasing the nodule count in a given cast iron leads to: Increasing strength and ductility in ductile cast iron [1]. Reduction of microsegregation of alloying elements [, 3], and improving microstructural homogeneity. Here, the type of eutectic transformation (stable or metastable) is also influenced due to the redistribution of alloying elements. Reduction in the chilling tendency of cast iron [4, 5]. Increasing preshrinkage expansion [6]. Increasing formation of open and closed contraction cavity volumes [7]. Increasing fraction of ferrite in the microstructure [8]. The chilling tendency (CT) of cast iron dictates their subsequent performance in diverse applications. In particular, cast iron possessing a high chilling tendency is prone to develop zones of white or mottled iron. Considering that, these regions can be extremely hard, their machinability can be severely impaired. Alternatively, if white iron is the desired structure a relatively small chilling tendency favours the formation of grey iron. This in turn leads to poor hardness and wear properties for the cast components. Hence, considerable efforts have been made in correlating various factors of technological relevance (inoculation practice, iron composition, pouring temperature, etc.) with the chill of cast iron. In this work, a simple analytical model of eutectic transformation in ductile cast iron is proposed. The model enables the determination of nodule counts in nodular cast iron, the chilling tendency CT and chill of ductile cast iron.. ANALYSIS Ductile cast iron is often hypereutectic, where the volume fraction of preeutectic graphite f gr is given by fgr ( C C ) ρl e = 100 ρgr Ceρ l + C( ρl ρgr) (1) where Ce = Si 0.36P () The influence of carbon and silicon on the preeutectic volume fraction of graphite is shown in Figure 1. From this figure it can be observed that for a useful C and Si range in the 116
5 foundry practice f gr ranges from 0 to 0.0; as a result, solidification of preeutectic graphite can be neglected. In this case, during solidification, heat extraction leads to changes in the relative energies of solid and liquid in two ways: 1) a reduction in the enthalpy of the liquid or solid due to cooling given by Ä H = cdt, ) a release heat of the eutectic solidification through the enthalpy contribution, known also as the latent heat (L). Hence, the heat transfer process can be described by the heat balance equation Fig. 1. Effect of carbon and silicon on the volumetric fraction of preeutectic graphite in hypereutectic cast iron qm = qs + qa (3) Heat transfer during solidification can be very complex and analytical solutions are not always available, so numerical methods are commonly employed. However, in sand castings, heat transfer is mainly determined by the properties of the sand mold as shown by Chvorinov [9]. a) b) T i a) mould b) Temperature T s T m I II ΔT m Temperature metal T i t s t m Time Fig.. Cooling curve for eutectic ductile cast iron (a) and temperature profile in the moldmetal system (b) Figure b shows the ideal temperature profile expected for sandmould metal systems. The heat flux going into the mold can be described by qm = Tkm ð á d t (4) 117
6 Taking into account the thermal diffusivity α d = k m /c m and the surface area F c of the casting, Eq. (4) can be rearranged as aft c qm = ð t (5) where a = k c. m m The above expression neglects curvature effects associated with the metalmold interface. Moreover, it is assumed that the temperature distribution along the metal is uniform. Hence, the accumulated heat flux in the metal can be described by cvc dt qa = dt (6) The heat flux q s generated during solidification depends on the particular solidification mechanism and in the present work it can be described by dv qs = LeNVc dt (7) where dv/dt is the volumetric solidification rate of eutectic cells (cm 3 /s). During solidification, two main stages can be distinguished (Fig. a). First Stage In this stage, the temperature of the melt decreases from T i to the equilibrium temperature for graphite eutetctic T s with no solidification events (Fig. a). Accordingly, q s = 0 and Eq. (3) can be rewritten as q m = q a (8) Taken into consideration Eqs. (5) and (6) and solving Eq. (8) for the initial conditions: T = T i at t = 0, the temperature during this stage is given by t T = Ti exp AM where: A = c π a (9) (10) M V = F c c (11) 118
7 Differentiating Eq. (9) yields an equation for the cooling rate as dt dt T i t = exp AM t A M (1) For t = t s, T = T s, and the time elapsed during the first stage can be found from Eq. (9) t s = (A B M) (13) where B = T ln i Ts (14) The metal cooling rate at the end of first stage can be calculated by taking into account Eqs. (1) (14) for t = t s, T = T s condition and after rearranging, yielding 1) dt Ts a = Q = dt (15) π Bc M Second Stage During this stage, the solidification of graphite eutectic occurs in the t s < t < t m time range or in the T s < T < T m temperature range (Fig. a). The initial segment of the cooling curve where the eutectic transformation takes place can be defined as a function of the degree of maximum undercooling ΔT m = T s T m (Fig. a). The solidification temperature for this temperature range can be described by [10] ( ) T = Ts ΔTmsin ω t ts (16) where ω= π ( t t ) m s (17) Equation (16) is of empirical nature. However it has been shown to provide an excellent description of the experimental outcome [10]. Accordingly, during second stage the cooling rate can be found by differentiating Eq. (16). dt dt = ΔTmωcos[ ω( t ts)] (18) 1) It is assumed that cooling rate has positive sign. 119
8 Therefore at the beginning of stage II when t = t s, cos0 = 1, the cooling rate can be described by ) dt Q = =ω Δ Tm (19) dt Combining Eqs. (17) and (19), and rearranging, yields ΔTm ( t t ) m s = Q π (0) At the onset of eutectic solidification (t = t s ), the cooling rates in the first and second stages it can be assumed equal each other. Therefore, using Eqs. (13), (15), and (0), the time for the maximum undercooling can be determined from t m ( +π Δ ) π Bc M BTs T = 4 a T s m (1) Nuclei N of nodular graphite are formed in the casting volume of liquid V c, and from each nucleus rise a single eutectic cell of spherical shape. Hence, the volume of the eutectic 3 cell with radius R (Fig. 3b) is given by V = (4 π R ) /3, while the differential volume increment is given by dv = 4 π R dr. Accordingly, taking into account Eq. (7) the expression for the rate of heat generation can be described by 4 π Le N Vc R dr q s = dt () In order to determine the radius R, as well as the growth rate of the cell, dr /dt the eutectic transformation in nodular cast iron will now be considered. Taking into account diffusional transport during the eutectic transformation and assuming spherical geometry (Fig. 3), the steady state solution for carbon diffusion through the austenite shell can be defined by solving equation dc d C D + = 0 rdr dr (3) ) It is assumed that cooling rate has positive sign. 10
9 a) b) Temperatue T s J ' E B C D graphite austenite R 1 R T ΔT m S C C 3 C 4 Carbon content C gr C 4 C C 3 Fig. 3. Schematic representation of a FeC phase diagram section (a) and corresponding carbon profile for a spherical eutectic cell (b) The general solution to the above equation yields ϕ C =ϕ+ r 1 (4) where r is the radial coordinate, R 1 < r < R and ϕ and ϕ 1 are constants which can be determined from the boundary conditions: C = C 3 at r = R and C = C at r = R 1. This yields: R1(C C 3) ϕ= C3 R R 1 RR 1 (C C 3) ϕ 1 = R R 1 (5) (6) Hence, taking into account Eqs. (4), (6) the solute concentration profile in the austenite envelope can be described by: ( C C )( ) R1 3 r R C( r) = C3 r ( R R1) (7) Moreover, deriving Eq. (7) with respect to r yields the carbon concentration gradient in the austenite envelope at the liquid austenite interface. dc R1 R (C C 3) = dr r ( R1 R) (8) 11
10 Also, at the austenite solidification interface r = R, the concentration gradient becomes dc R1(C3 C ) = dr R R R ( ) 1 (9) Introducing a mass balance in the diffusional system (Fig. 3b) where (C 4 ) is the carbon content in the volume (4πR 3 )/3 prior to the eutectic transformation (when only liquid is the stable phase). In this case, the mass of carbon in the liquid can be given by ml 4 3 = π R C4 (30) 3 After the eutectic transformation, the diffusional system is depicted by a graphite nodule of radius R 1 and concentration C gr surrounded by an austenite envelope of radii R 1 and R. The mass of carbon in the graphite nodule can be determined from mgr 4 3 = π R1 Cgr (31) 3 A differential increment in the volume of the austenite envelope dv = 4πr dr causes a differential increment in the carbon mass according to dm γ = 4 π C( r) r dr (3) Also, the carbon mass in the austenite envelope is described by R R1 mγ = 4 π C() r r dr (33) Considering Eqs. (7) and (33) and rearranging terms yields mγ = π C3R C R1 R1 R(C3 C )( R R1) 3 + (34) In the above equation, the third term within brackets is relatively small and can be neglected. This yields 3 3 ( C3 C 1 ) 4 mγ = R R 3 π (35) 1
11 From the mass balance (m l = m gr + m γ ), based on Eq. (30), (31) and (35) R 1 is found as 1/3 C4 C R 3 1 R = Cgr C (36) In addition, the condition for continuity across the liquid austenite interface needs to be taken into account. This condition using Fick law can be written as (C 4 dr dc C 3) D dt = dr (37) Combining Eqs. (9), (36), and (37) yields RdR = kddt (38) where k = ( ) (C C ) 3 C C gr C4 C3 3 1 C4 C3 (39) The above expression can be correlated with the degree of undercooling, ΔT. Assuming that the JE, E S and BC lines for the FeC system (Fig. 3a) are straight the concentrations in Eq. (39) can be given by: ΔT C = C E ' (40) m ΔT C3 = C E ' + (41) m 3 ΔT C4 = C C ' + (4) m 4 where: m, m 3 and m 4 are the slopes of the solubility lines JE, E S and BC respectively. 13
12 For FeC alloys the following values can be employed: C C = 4.6%, C E =.08%, m = 75 o C / %, m 3 = o C / %, and m 4 = = 113. o C / %. Using this data, estimations of k values are plotted in Figure 4. From this figure, it is apparent that k tends to exhibit a linear trend with ΔT. Accordingly, k can be described by k = β ΔT (43) where β = o C 1. Moreover, it can be shown that the effect of Si on β is negligible. In addition, considering that the degree of undercooling ΔT = T s T, from Eqs. (16), (38) and (43), it is found that Fig. 4. Graphic plot of Eq. (39) function as a function of the degree of undercooling, ΔT ( ) R dr =βd ΔTmsin ω t ts dt (44) Hence, integrating the above expression for the limiting conditions t = t s at R = 0, yields β D ΔT R m = 1 cos ω t ts ω ( ) 1/ (45) Differentiating Eq. (45) with respect to time yields the rate of eutectic cell growth 1/ dr β D ωδt m = sin ω( t ts ) dt 1 cos ( t t ω s ) (46) Then, at the time t = t m, and by taking into account Eq. (17), expressions for the cell radius, as well as the cell growth rate at the maximum undercooling are found: 1/ β D ΔT R m, m = ω (47) 1/ dr, m β D ω ΔTm = dt (48) 14
13 In addition, by taking into account Eqs. (10), (13), (17), (1), (), (47) and (48), the heat flux generated during solidification at the time t = t m is given by cm qs = 4 LeN Vc a ( ) B ΔTm π β D ΔTm T s 3 1/ (49) Moreover, combining Eqs. (3) and (1) for the same time t = t m, the heat flux going into the mold can be described by 3/ Fc a T q s m = 1/ 1/ π cm B ( π Δ Tm + Ts B) (50) At t = t m, the cooling rate is zero and as a consequence the rate of heat accumulation q a is also zero. Hence, the heat balance equation (Eq. (3)) becomes qs = qm (51) Finally, by taking into account Eqs. (11), (1), (49) and (51) an expression for the modulus of casting can be obtained. M 1/3 a T s = 1/ 5/ 1/ ( Dβ) π BNLe c ΔTm ( π Δ Tm + TB s ) (5) In nodular cast iron, the pouring temperature, T p ranges from 150 to 1450 o C. Hence, taking into account that T p = T i, typical B values (Eq. (14)) range from to 0.3. Figure 5 shows graphically the ( ) 1/ 1/ ΔTm π Δ Tm + TsB and z Δ TmTs functions versus ΔT m for two extreme values of B. From this figure it is evident that ( ) 1/ m m s s 1/ m ΔT π Δ T + T B z T Δ T (53) where z = B (54) Accordingly, taking into account Eqs. (5) and (53), N can be simplified to the following form M 1/ Ts 1 = a D 5/ β π zbnleδt m 1/3 (55) 15
14 a) b) m m s Δ π Δ + (solid line) and line) functions for: a) B = 0.074; b) B = 0.3 Fig. 5. Influence of ΔT m and B on the T ( T B T ) 1/ 1/ z Ts Δ Tm (dotted 3. NODULE COUNT Eq. (55) can be rewritten as a function of the cooling rate (taking into account Eq. (15)) as 1/ cb Q N = 1/ 4 π z L D e ΔT β m 3/ (56) The nucleation of graphite during solidification is of heterogeneous nature, on preferential substrates of various sizes, l s. The active substrate set is randomly distributed in the undercooled melt and it can be given by the substrate volume density, N s. A simple heterogeneous nucleation model previously developed [11] is employed in this work. Accordingly, the volume density of graphite nodules can be given by b N = Ns exp ΔT m (57) where 4 Ts σ sin θ b = Le l (58) Combining Eqs. (56) and (57) yields 1/ b c B Q Ns exp = ΔT π Δ D β 1/ m 4 z Le Tm 3/ (59) From this equation, the maximum degree of undercooling can be determined from Δ Tm = b ProductLog ( y) (60) 16
15 where 1/ 3 3 1/4 π zns Le D β y = b c 3 BQ (61) The ProductLog[y] = x is the Lambert function 3), also is called the omega function and it is graphically shown in Figure 6. This function is used to solve equation of the x type of y = xe. Its exact values can be easily calculated using the instruction of the ProductLog[y] in the Mathematica programme. In our analysis typical values of variable y are situated within boundaries from 0.03 to 500, and in case if we cannot Fig. 6. Graphic representation of the ProductLog[y] function for y 0 use Mathematica programme its value can be calculated by means of elementary mathematics with an accuracy higher than 99% using the following equations: for 0.03 y 1 range y x = ; y y for 1 y 5 range x= log( ) y y ; for 5 y 0 range x= log( ) y y ; for 0 y 50 range x= log( ) y y ; for 0 y x= log( ) y y. From Eqs. (57) and (60) N can be given by N N = s exp ProductLog( y) In metallographic determinations, the area density of graphite nodules N F is commonly measured at a given microsection. In addition, in ductile iron the graphite nodules are cha (6) 3) See 17
16 racterized by Raleigh distributions [1]. In this case the volumetric nodule count (N) can be related to the area nodule count (N F ) using the Wiencek equation [13] ( ) 1/3 gr NF = f N (63) where f gr is the volume fraction of graphite in eutectic, f gr = According to the literature, the nodule count N F is influenced by the chemical composition and the superheat temperature and time [14]. Yet, in the industrial practice, a drastic increase in nodule counts is usually obtained by the introduction of inoculants. In this case, the nodule count depends on the type of inoculant, quantity and granulation, Mg treatment and inoculation temperature, and the time after inoculation [14]. Also, it is well known that an increase in the cooling rates causes a radical increase in the nodule count in castings. From Eqs. (60) and (61) it can be seen that among the various factors that influence the final nodule count are: The diffusion coefficient of carbon in austenite, D depends on the actual temperature and chemical composition of the austenite. The effect of Si, Mn and P on D is not considered in this work as there is not enough information available in the literature. An expression for the diffusion coefficient of carbon in austenite has been published [15] D = exp , cm /s T T (64) During the eutectic transformation, the temperature, T ranges from to K, so the effective D values ranges from to cm /s. Therefore, an average D value of cm /s can be used without introducing significant error. In general, as D increases, the nodule count decreases as predicted by Eqs. (61) (11), (also see Fig. 7). Nucleation susceptibilities. Depending on the graphite nucleation susceptibilities in ductile cast iron at a given cooling rate, various nodule counts can be achieved. The nucleation susceptibilities of cast iron (Tab. 1) are characterized by N s and b. These coefficients (see Tab. 4, Part II) depend on the chemical composition, spheroidization practice, inoculation, and holding time of bath and temperature. Fig. 7. Influence of the diffusion coefficient for carbon in austenite on the nodule count; L e = 08.8 J/cm 3 ; c = 5.95 J/(cm 3 oc); β = o C 1 ; C = 3.71%, Si =.77%, P = 0.034%; T i = 1300 o C; D = = cm /s (rest of data see Tab. 1) 18
17 Table 1. Physicalchemical data for nodular cast iron Latent heat of graphite eutectic L e = 08.8 J cm 3 Specific heat of the cast iron Coefficient of heat accumulation by the mould material c = 5.95 J cm 3 o C a = 0.1 J cm s 1/ o C Diffusion coefficient of carbon in austenite D = cm s 1 Coefficient β = o C 1 Equilibrium temperature of the graphite eutectic Cementite eutectic formation temperature ΔT sc = T s T c T s = Si 14.88P T c = (C 3.33Si 1.58P), o C ΔT sc = C Si +36.9P, o C Eutectic density ρ e = 0.96ρ γ ρ gr, g cm 3 Austenite density ρ γ = 7.51 g cm 3 Graphite density ρ gr =. g cm 3 Melt density ρ l = 7.1 g cm 3 Average temperature of the metal just after pouring in the mold cavity T i = 150 o C The influence of the nucleation coefficients on the nodule count is shown in Figure 8. The calculations made for nodule count were based on Eqs. (61) (63). From Figure 8, it is apparent that the nodule count increases when b decreases and N s increases. In addition, it is well known [11] that for given cooling rate prolonged bath holding time leads to reduction in N s and to an increase in b parameter. Consequently, prolonged bath holding time leads to a reduction in the nodule count. According to Eq. (15) the cooling rate increases as the ability of the mold to absorb heat a increases and as the casting modulus M decreases. The cooling rate is also dependent on the B parameter (Eq. 14), and hence on the initial temperature T i of the cast iron just after pouring into the mould. It also depends on the equilibrium eutectic temperature T s and the specific heat c (Eq. (15). Figure 9 shows the effect of B and of the a/m ratios on the cooling rate at the onset of eutectic solidification. A schematic diagram showing the role of various technological factors on the nodule count in ductile cast iron is given in Figure
18 a) b) Fig. 8. Influence of the nucleation coefficient on the nodule count: a) N s = cm 3 ; b) b = 60 o C (rest of data see Fig. 7) Fig. 9. Effect of B (T i, T s ) and a/m ratio on the cooling rate Q 130
19 Nodule count N Cooling rate Q Diffusion coefficient D Nucleation coefficients N s, b Initial temperature of melt T i Casting modulus M Mould material a Chemical composition of bath Furnace slag and atmosphere Spheroidizing and inoculation practice Temperature and holding time of bath Technological factors Fig. 10. Effect of technological factors on the nodule count in ductile cast iron 4. CHILLING TENDENCY Since ΔT m = T s T m, a plot of the function T m = f (Q) using Eqs. (60) and (61) is given in Figure 11. From this figure, it is found that the minimum temperature for the solidification of the graphite eutectic T m levels with the temperature T c when the cooling rate, Q = Q cr and ΔT m = T s T c = ΔT sc, so below T c, the solidification of cementite eutectic begins. By taking into account this condition into Eqs. (60) and (61) and using Eq. (15) an expression is derived for the critical casting modulus M cr = (V/F) cr below which a chill is likely to develop in castings Mcr = pcr CT (65) where the coefficient p cr includes the parameters (a, z, B T s ) related to the cast iron cooling rates 4) p cr 3 T s = a π β z B Le c 1/6 (66) 4) Influence of L e and c can be neglected. 131
20 Fig. 11. Influence of the cooling rate Q on the minimal solidification temperature T m for graphite eutectic (rest of data see Fig. 7) CT is the chilling tendency for ductile cast iron 1 1 b CT = exp 1/ D N T s βδt Δ sc sc 1/3 (67) From Eqs. (57) and (67), for ΔT m = ΔT sc, CT can be simplified to 1/3 1 1 CT = 1/ D N T βδ sc (68) Typical CT values range from 0.8 to 1. s 1/ / o C 1/3. The influence of the various terms on CT, (Eq. (68)) can be summarized as: Diffusion coefficient, as D increases, CT decreases. The temperature range ΔT sc = T s T c, depends on the chemical composition as o Δ = C Si P, C (69) T sc In particular, carbon reduces ΔT sc while silicon expends it (Fig. 1a). The effect of this range on CT is shown in Figure 1b. Notice from this figure that CT decreases with increasing ΔT sc ranges. The Nucleation susceptibilities of graphite depends on the resultant values of N s and b (see previous section). In particular, CT increases with increasing b and decreasing N s (Fig. 13). 13
21 a) b) Fig. 1. Influence of carbon and silicon on: a) ΔT sc ; b) ΔT sc on the chilling tendency CT Fig. 13. Influence of N s and b on the chilling tendency of ductile cast iron; ΔT sc = 60 o C (rest of data see Fig. 7) 5. CHILL In establishing the chill of cast iron, it is common to implement a set of chill tests on castings, which consist of plates with different wall thicknesses, thus the critical casting modulus can be determined from M cr V = F cr cr (70) where V cr and F cr are chilled volume and surface area of casting. 133
22 Clill s cr Influence on cooling rate Temperature range ΔT ec Chilling tendency CT Diffusion coefficient D Nodule count N Nucleation parameters N s, b Initial temperature of melt T i Mould Material a Eutecic temperature T e Chemical composition of bath Furnace slag and atmosphere Spheroidizing and inoculation practice Temperature and holding time of bath Technological factors Fig. 14. Effect of technological factors on the chill and chilling tendency of ductile iron For plates with wall thickness, s and lengths and widths which easily exceed s, M cr = = V cr /F cr = (s cr F cr )/( F cr ), and the critical wall thickness s cr below which the chill forms is scr = Mcr (71) and after using Eq. (65) scr = pcr CT (7) From Eqs. (66), (67) and (7) results a diagram showing the influence of technological factors on chilling tendency CT and the chill of ductile cast iron is shown in Figure CONCLUSIONS A theoretical analysis is proposed for the solidification of ductile cast iron which allows to predict nodule counts based only on the knowledge of cooling rates and chemical composition, the initial temperature of the metal just after pouring into the mould, the diffu 134
23 sion coefficient of carbon in austenite and the graphite nucleation coefficients. From the proposed theory, expressions are derived for the chilling tendency and chill of cast iron. A summary of the present analysis on the nodule count of cast iron indicates that it depends on: The chemical composition of the cast, through D, N s, and b. The inoculation practice, the bath superheating temperature and time, furnace slag and atmosphere, through N s and b. Cooling rate, through M, a and B. The chilling tendency CT of the nodular cast iron depends on: Chemical composition through D, ΔT sc, N s, and b, Inoculation and spheroidization practice, superheat temperature and time, as well as furnace slag and atmosphere through N s and b. In addition, the chill of the nodular cast iron is related to cooling rate Q and CT. REFERENCES [1] Jincheng Liu, Elliot R.: The influence of cast structure on the austempering of ductile iron. International Journal of cast Metals Researches, 11 (1999), p. 407 [] Lesoult G., Castro M., Lacaze J.: Solidification of Spheroidal Graphite Cast Iron: III Microsegregation related effects. Acta Materialia, 47 (1999), p [3] Achmadabadi M.N., Niyama E., Ohide T.: Structural control of 1% Mn aided by modeling of microsegregation. Transactions of the American Foundrymans Society, 97 (1994), p. 69 [4] Javaid A., Thompson J., Davis K.G.: Critical conditions for obtaining carbide free microstrucutre in thinwall ductile iron. AFS Transactions, 10 (00), p. 889 [5] Javaid A., Thompson J., Sahoo M., Davis K.G.: Factors affecting formation of carbides in thinwll DI castings, AFS Transactions, 99 (1999), p. 441 [6] Fraœ E., Lopez H.: Generation of International Pressure During Solidification of Eutectic Cast Iron. Transactions of the American Foundryman Society, 10 (1994), p. 597 [7] Fraœ E., Podrzucki C.: Inoculated Cast Iron. AGH, Cracov, 1981 [8] Venugopalan D.: A Kinetic Model of the γ α + Gr Eutectoid Transformation in Spheroidal Graphite Cast Iron. Metallurgical and Materials Transactions, 1 A (1990), p. 913 [9] Chvorinov N.: Theorie der Erstarrung von Gusstûcken. Die Giesserei (1940) 7, p. 10 [10] Fras E., Lopez H.: A theoretical analysis of the chilling suspectibility of hypoeutectic FeC alloys. Acta Metallurgica and Materialia, 41 (1993) 1, p [11] Fras E., Górny M., Lopez H., Tartera J.: Nucleation and grains density in grey cast iron. A theoretical model and experimental verification. International Journal of Cast Metals Research, 16 (003), pp [1] Wojnar L.: Effect of graphite size and distribution on fracture and fractography of ferritic nodular cast iron. Acta Stereologica, 5/ (1986), p
24 [13] Wiencek K., Ryœ J.: The estimation of Fe 3 C particle density in steel by simple counting measurements made in plan sections. Materialas Engineering (1998) 3, p. 396 [14] Merchant H.D.: Solidification of Cast Iron, Recent Research on Cast iron. Gordon and Breach, Science Publishers, NewYork, 1968 [15] Agren J.: A revised expression for the diffusivity of carbon in binary FeC austenite. Scripta Metallurgica, 0 (1986), p Received March
Production of ductile iron castings without feeders
Production of ductile iron castings without feeders Possibilities of producing ductile iron castings in green sand mould without feeders by means of "ingate" feeding and control of the graphite precipitation
More informationCalorimetric analysis of heating and cooling process of nodular cast iron
ARCHIVES of FOUNDRY ENGINEERING Published quarterly as the organ of the Foundry Commission of the Polish Academy of Sciences ISSN (18973310) Volume 7 Issue 1/2007 25 30 5/1 Calorimetric analysis of heating
More information= 62 wt% Ni38 wt% Cu.
92 9.2 (a) From Figure 9.8, the maximum solubility of Pb in Sn at 100 C corresponds to the position of the β (α + β) phase boundary at this temperature, or to about 2 wt% Pb. (b) From this same figure,
More informationTHE INFLUENCE OF IRON POWDER AND DISINTEGRATED STEEL SCRAP ADDITIVES ON THE SOLIDIFICATION OF CAST IRON
METALLURGY AND FOUNDRY ENGINEERING Vol. 36, 2010, No. 2 Dariusz Kopyciñski*, Józef Dorula** THE INFLUENCE OF IRON POWDER AND DISINTEGRATED STEEL SCRAP ADDITIVES ON THE SOLIDIFICATION OF CAST IRON 1. INTRODUCTION
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationInoculation of Cast Irons An Overview
Inoculation of Cast Irons An Overview J.N. Harvey and G.A. Noble J.N. Harvey Tennant Metallurgical Group Ltd, Chesterfield, United Kingdom G.A. Noble Tennant Metallurgical Group Ltd, Chesterfield, United
More informationComposition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)
10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationSolution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.
14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius
More informationLecture 19: Eutectoid Transformation in Steels: a typical case of Cellular
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
More informationCast Iron Foundry Practices 4. Grey iron foundry practices
MME 345, Lecture 37 Cast Iron Foundry Practices 4. Grey iron foundry practices Ref: [1] Heine, Loper and Rosenthal. Principles of Metal Casting, Tata McGrawHill, 19670 [2] J R Brown (ed.). Foseco Ferrous
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More informationSOLIDIFICATION. (a)formation of stable nuclei. Growth of a stable nucleus. (c) Grain structure
SOLIDIFICATION Most metals are melted and then cast into semifinished or finished shape. Solidification of a metal can be divided into the following steps: Formation of a stable nucleus Growth of a stable
More informationKinetics of Phase Transformations: Nucleation & Growth
Kinetics of Phase Transformations: Nucleation & Growth Radhika Barua Department of Chemical Engineering Northeastern University Boston, MA USA Thermodynamics of Phase Transformation Northeastern University
More informationMetal Expansion Penetration on Concave Casting Surfaces of Grey Cast Iron Cylinder Heads
Metal Expansion Penetration on Concave Casting Surfaces of Grey Cast Iron Cylinder Heads Izudin Dugic, Attila Diószegi and Ingvar L Svensson Research report 2006:1, ISSN 14040018 Jönköping University
More informationLecture: 33. Solidification of Weld Metal
Lecture: 33 Solidification of Weld Metal This chapter presents common solidification mechanisms observed in weld metal and different modes of solidification. Influence of welding speed and heat input on
More informationDesign of Cast Parts Avoid sharp corners, angles & fillets They act as stress raisers Select fillet radii to reduce stress concentrations and ensure p
Metal Casting Design, Materials, Economics Text Reference: Manufacturing Engineering and Technology, Kalpakjian & Schmid, 6/e, 2010 Chapter 12 Design of Cast Parts Avoid sharp corners, angles & fillets
More informationUNIVERSITY OF CALIFORNIA College of Engineering Department of Materials Science & Engineering MSE 121. Spring Semester 2008 Professor R.
UNIVERSITY OF CALIFORNIA College of Engineering Department of Materials Science & Engineering MSE 121 Spring Semester 2008 Professor R. Gronsky Exam Instructions Please PRINT your name in the box above
More information9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure
913 9.8: 9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure (a) The first liquid forms at the temperature at which a vertical line at this composition
More informationModule 34. Heat Treatment of steel IV. Lecture 34. Heat Treatment of steel IV
Module 34 Heat reatment of steel IV Lecture 34 Heat reatment of steel IV 1 Keywords : Austenitization of hypo & hyper eutectoid steel, austenization temperature, effect of heat treatment on structure &
More informationEFFECT OF SECTION SIZE ON PRODUCING DUCTILE IRON CASTINGS
2/13 Archives of Foundry, Year 4, Volume 4, 13 Archiwum Odlewnictwa, Rok 4, Rocznik 4, Nr 13 PAN Katowice PL ISSN 1642538 EFFECT OF SECTION SIZE ON PRODUCING DUCTILE IRON CASTINGS S. BOCKUS 1, A. DOBROVOLSKIS
More informationChapter 10: Phase Transformations
Chapter 10: Phase Transformations ISSUES TO ADDRESS... Transforming one phase into another takes time. Fe C FCC γ (Austenite) Eutectoid transformation Fe 3 C (cementite) + α (ferrite) (BCC) How does the
More informationIntroduction to Iron Metallurgy. Lee Morin Houston Home Metal Shop Club October 2010
Introduction to Iron Metallurgy Lee Morin Houston Home Metal Shop Club October 2010 Book I stole the pictures from We will start with a brief overview! Metals Are Crystals Fundamental geometry of a crystal
More informationMultiPhase MicroSegregation Modelling during Solidification of Ductile Iron
MultiPhase MicroSegregation Modelling during Solidification of Ductile Iron B. Pustal, R. Berger, E. Subasic, G. Laschet, W. Schäfer, C. Bartels, A. BührigPolaczek Prof. Dr. Ing. A. BührigPolaczek
More informationAvoiding Shrinkage Defects and Maximizing Yield in Ductile Iron
Paper 12081.pdf, Page 1 of 16 Avoiding Shrinkage Defects and Maximizing Yield in Ductile Iron D. White Elkem Metals, Inc, Boca Raton, FL USA Copyright 2012 American Foundry Society ABSTRACT The presentation
More informationIntroduction to Materials Science, Chapter 9, Phase Diagrams. Phase Diagrams. University of Tennessee, Dept. of Materials Science and Engineering 1
Phase Diagrams University of Tennessee, Dept. of Materials Science and Engineering 1 Chapter Outline: Phase Diagrams Microstructure and Phase Transformations in Multicomponent Systems Definitions and basic
More informationPhase transformation
Phase transformation Phase Transformation Topics o Basic principles relating to transformations o Kinetics of phase transformation: Nucleation and growth o Metastable and equilibrium state o Shape memory
More informationCOMPUTER SIMULATION BASED COMPARATIVE STUDY ON THE SOLIDIFICATION OF A CAST IRON AND STEEL CASTING
COMPUTER SIMULATION BASED COMPARATIVE STUDY ON THE SOLIDIFICATION OF A CAST IRON AND STEEL CASTING Aurel CRIŞAN*, Ioan CIOBANU*, Daniela IONESCU*, Maria STOICĂNESCU* *Transilvania University of Braşov,
More informationEffect of atmosphere in a foundry mould on casting surface quality
ARCHIVES of FOUNDRY ENGINEERING Published quarterly as the organ of the Foundry Commission of the Polish Academy of Sciences ISSN (18973310) Volume 12 Issue 1/2012 13 18 3/1 Effect of atmosphere in a
More informationModule 4 Design for Assembly IIT BOMBAY
Module 4 Design for Assembly Lecture Design for Heat Treatment 7 Instructional objectives By the end of this lecture, the student will learn 1. different heat treatment processes, 2. application of various
More informationMIT 2.810 Manufacturing Processes and Systems. Homework 6 Solutions. Casting. October 15, 2015. Figure 1: Casting defects
MIT 2.810 Manufacturing Processes and Systems Casting October 15, 2015 Problem 1. Casting defects. (a) Figure 1 shows various defects and discontinuities in cast products. Review each one and offer solutions
More informationMAE 20 Winter 2011 Assignment 3 solutions
MAE 20 Winter 2011 Assignment 3 solutions 4.3 Calculate the activation energy for vacancy formation in aluminum, given that the equilibrium number of vacancies at 500 C (773 K) is 7.57 10 23 m 3. The
More informationBURNON SURFACE DEFECTS OF IRON CASTINGS
BURNON SURFACE DEFECTS OF IRON CASTINGS JÓZSEF TAMÁS SVIDRÓ University of Miskolc, Department of Metallurgical and Foundry Engineering 3515 Miskolc, Egyetemvaros fridoline@freemail.hu The right surfacial
More informationComparison of Three NiHard I Alloys
Comparison of Three NiHard I Alloys Ö. N. Do an 1, J.A. Hawk 1, and J.Rice 2 1 U.S. Department of Energy, Albany Research Center, Albany, Oregon 2 Texaloy Foundry Co., Inc., Floresville, Texas Keywords:
More informationLecture 7: Oxidation of manganese and carbon. Key words: Solidification of steel, decarburization, BOF steelmaking
Lecture 7: Oxidation of manganese and carbon Contents: Behaviour of manganese Oxidation of manganese Reduction of manganese Oxidation of carbon Rimming reaction Illustration Key words: Solidification of
More informationProblem Set 7 Materials101 1.) You wish to develop a gold alloy (mostly gold) that can be precipitation strengthened to provide high strength  high conductivity electrical leads to integrated circuits
More informationSolidification. Strength and Movement of Solid. Cast Iron in the Sand Mold*
UDC 669.13:621.746.62:539.32.096 Strength and Movement of Solid Skin during Solidification of Cast Iron in the Sand Mold* By Tatsushi AIZAWA** and Akihide WA TANABE** Synopsis The strength of the solid
More informationContinuous Cooling Transformation (CCT) Diagrams
Continuous Cooling Transformation (CCT) Diagrams R. Manna Assistant Professor Centre of Advanced Study Department of Metallurgical Engineering Institute of Technology, Banaras Hindu University Varanasi221
More informationPOURING THE MOLTEN METAL
HEATING AND POURING To perform a casting operation, the metal must be heated to a temperature somewhat above its melting point and then poured into the mold cavity to solidify. In this section, we consider
More informationHigh Temperature Thermal Fatigue Property of ThinSection Ductile Cast Iron
Paper 10056.pdf, Page 1 of 12 High Temperature Thermal Fatigue Property of ThinSection Ductile Cast Iron Copyright 2010 American Foundry Society E. N. Pan, C. C. Fan, H. Y. Chang National Taiwan University,
More informationSteel and cast iron. Chapter Chapter 112
Steel and cast iron Chapter 111 Chapter 112 1 Taxonomy of Metals Metal Alloys Ferrous Steels Cast Irons
More informationThe transformation of the foundries in complex. New approach to process control in cast iron foundries through thermal analysis
New approach to process control in cast iron foundries through thermal analysis ANDREA ZONATO a1 1 ProService Srl, Massanzago (PD) ITALY, www.proservicetech.it, www.itaca8.com Abstract The continuous increase
More informationDefect formation in cast iron
Defect formation in cast iron School of Engineering Jönköping University Sweden Tammerfors, Finland, November 8, 2012 Introduction Casting Mould cavity Melting process Pouring Solidification Mould removal
More informationDevelopment of Mathematical Equation for Fraction of Solid in AlSi7Mg Alloy Solidification Simulation
Journal of Minerals & Materials Characterization & Engineering, Vol. 7, No.1, pp 718, 007 jmmce.org Printed in the USA. All rights reserved Development of Mathematical Equation for Fraction of Solid in
More informationPrediction of Solidification Time: Chvorinov's Rule.
Prediction of Solidification Time: Chvorinov's Rule. The amount of heat that must be removed from a casting to cause it to solidify is directly proportional to the amount of superheating and the amount
More informationHIGH STRENGTH DUCTILE IRON PRODUCED BY THE ENGINEERED COOLING: PROCESS CONCEPT
IJMC142442 HIGH STRENGTH DUCTILE IRON PRODUCED BY THE ENGINEERED COOLING: PROCESS CONCEPT Copyright 215 American Foundry Society Abstract Simon N. Lekakh Missouri University of Science and Technology,
More informationHW 8. G = a 3 G v. 6a 2. Problem a. To Find:
HW 8 Problem 10. a. To Find: (a) The expression for total free energy change for a cubic nucleus, critical cube edge length, a*, and G* (b) Compare G* for a cube with that for a sphere b. Given: Nucleus
More information3. Apply phase rule to the two phase field of a binary isomorphous diagram. What conclusion can be drawn?
ecture 1822: Solidification of binary alloys: Solidification of binary alloys: limits of solubility, isomorphous system, lever rule, constitutional super cooling, effect of non equilibrium cooling, eutectic,
More informationLecture 4: Thermodynamics of Diffusion: Spinodals
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP6, Kinetics and Microstructure Modelling, H. K. D. H. Bhadeshia Lecture 4: Thermodynamics of Diffusion: Spinodals Fick
More informationSteady Heat Conduction
Steady Heat Conduction In thermodynamics, we considered the amount of heat transfer as a system undergoes a process from one equilibrium state to another. hermodynamics gives no indication of how long
More informationSimulations of the Effect of Section Size and Cooling on Sigma Phase Formation in Duplex Stainless Steels
Simulations of the Effect of Section Size and Cooling on Sigma Phase Formation in Duplex Stainless Steels Richard A. Hardin and Christoph Beckermann Department of Mechanical and Industrial Engineering
More informationTHREE MAIN SOLIDIFICATION REACTIONS OF VANADIUM MODIFIED T1 TUNGSTEN HIGH SPEED TOOL STEEL. Hossam Halfa
THREE MAIN SOLIDIFICATION REACTIONS OF VANADIUM MODIFIED T1 TUNGSTEN HIGH SPEED TOOL STEEL Hossam Halfa Steel Technology Department, Central Metallurgical R&D Institute (CMRDI), Helwan, Egypt, hossamhalfa@cmrdi.sci.eg;
More informationDEVELOPMENT OF A LOW MELTING POINT WHITE CAST IRON FOR USE IN COMPOSITE ALLOY MANUFACTURE
MATERIALS FORUM VOLUME 312007 Edited by J.M. Cairney and S.P. Ringer Institute of Materials Engineering Australasia DEVELOPMENT OF A LOW MELTING POINT WHITE CAST IRON FOR USE IN COMPOSITE ALLOY MANUFACTURE
More informationDr. Alaa A. The Iraqi Journal For Mechanical And Material Engineering, Vol. 10,No. 1, 2010
Dr. Alaa A. The Iraqi Journal For Mechanical And Material Engineering, Vol. 10,No. 1, 2010 1.1 Metallurgy of gray cast iron: Most of industrial automobiles companies produced the brake rotor part from
More informationA Solutal Interaction Mechanism for the ColumnartoEquiaxed Transition in Alloy Solidification
A Solutal Interaction Mechanism for the ColumnartoEquiaxed Transition in Alloy Solidification M.A. MARTORANO, C. BECKERMANN, and Ch.A. GANDIN A multiphase/multiscale model is used to predict the columnartoequiaxed
More informationChapter 1 Introduction to Material science & Metallurgy
Chapter 1 Introduction to Material science & Metallurgy 1. Material Science & Metallurgy (21419) State the importance of study of materials science and briefly. Explain Engineering requirements of materials.
More informationUniversity of Cambridge, Materials Science & Metallurgy. Dilatometry
University of Cambridge, Materials Science & Metallurgy H. K. D. H. Bhadeshia Dilatometry The dilatometric method utilises either transformation strains or thermal strains; the basic data generated are
More informationHeat Treatment of Steel
Heat Treatment of Steel Steels can be heat treated to produce a great variety of microstructures and properties. Generally, heat treatment uses phase transformation during heating and cooling to change
More informationIntroduction to Materials Science, Chapter 11, Thermal Processing of Metal Alloys. Chapter 11 Thermal Processing of Metal Alloys
Chapter 11 Thermal Processing of Metal Alloys Designer Alloys: Utilize heat treatments to design optimum microstructures and mechanical properties (strength, ductility, hardness.) Strength in steels correlates
More informationSTUDY OF PROCESS PARAMETERS OF GRAVITY DIE CASTING DEFECTS
International Journal of Mechanical Engineering and Technology (IJMET) Volume 7, Issue 2, MarchApril 2016, pp. 208 211, Article ID: IJMET_07_02_023 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=7&itype=2
More informationIn order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More informationChapter 8. Phase Diagrams
Phase Diagrams A phase in a material is a region that differ in its microstructure and or composition from another region Al Al 2 CuMg H 2 O(solid, ice) in H 2 O (liquid) 2 phases homogeneous in crystal
More informationThe mechanical properties of metal affected by heat treatment are:
Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.
More informationAnalysis and Optimization of Investment Castings to Reduce Defects and Increase Yield
Analysis and Optimization of Investment Castings to Reduce Defects and Increase Yield Arunkumar P 1, Anand.S.Deshpande 2, Sangam Gunjati 3 1 Associate Professor, Mechanical Engineering, KLS Gogte Institute
More informationEstimating the Eutectic Composition of Simple Binary Alloy System Using Linear Geometry
Estimating the Eutectic Composition of Simple Binary Alloy System Using Linear Geometry Muhammed Olawale Hakeem AMUDA * and Raymond Otito AKABEKWA Department of Metallurgical and Materials Engineering
More informationChapter 5: Diffusion. 5.1 SteadyState Diffusion
: Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationHeat Treatment of Steels : Spheroidize annealing. Heat Treatment of Steels : Normalizing
Heat Treatment of Steels :Recrystallization annealing The carbon and alloy steels were treated at a temperature of about 700 C, which is about 20 C below the eutectoid temperature. The holding time should
More informationSolidification, Crystallization & Glass Transition
Solidification, Crystallization & Glass Transition Cooling the Melt solidification Crystallization versus Formation of Glass Parameters related to the formaton of glass Effect of cooling rate Glass transition
More informationAn Analysis of Heat Conduction with Phase Change during the Solidification of Copper
An Analysis of Heat Conduction with Phase Change during the Solidification of Copper J. Michalski and E. GutierrezMiravete *2 1 Hamilton Sundstrand, 2 Rensselaer at Hartford *Corresponding author: 275
More informationEffect of Section Thickness On The Microstructure And Hardness Of Gray Cast Iron (A Simulation Study)
Effect of Section Thickness On The Microstructure And Hardness Of Gray Cast Iron (A Simulation Study) Shrikant Sahu 1, Mohd. Nadeem Bhat 2, Ajit kumar 3,Avinaw Pratik 4, Amitesh kumar 5 Department of Foundry
More informationDer Einfluss thermophysikalischer Daten auf die numerische Simulation von Gießprozessen
Der Einfluss thermophysikalischer Daten auf die numerische Simulation von Gießprozessen Tagung des Arbeitskreises Thermophysik, 4. 5.3.2010 Karlsruhe, Deutschland E. Kaschnitz Österreichisches GießereiInstitut
More informationSolder Materials. Introduction
Solder Materials Introduction Most assemblies currently use solder in order to create connections between components and the printed circuit board. There was an indication in Polymer applications within
More informationPOSSIBILITY OF INDIRECT HARDNESS TESTING OF DUPLEX STAINLESS STEEL
1 POSSIBILITY OF INDIRECT HARDNESS TESTING OF DUPLEX STAINLESS STEEL István Mészáros Associate professor, Department of Materials Science and Engineering H1111 Budapest, Goldmann tér 3. Summary In this
More informationInfluence of Steel Scrap on Microstructure and Mechanical Properties of Spheroidal Graphite Cast Iron
Materials Transactions, Vol. 44, No. 7 (2003) pp. 1419 to 1424 #2003 The Japan Institute of Metals Influence of Scrap on Microstructure and Mechanical Properties of Spheroidal Graphite Cast Iron Sadato
More informationAlloys & Their Phase Diagrams
Alloys & Their Phase Diagrams Objectives of the class Gibbs phase rule Introduction to phase diagram Practice phase diagram Lever rule Important Observation: One question in the midterm Consider the Earth
More informationDetermination of Molecular Weight by Freezing Point Depression
Determination of Molecular Weight by Freezing Point Depression Freezing point depression is a kind of colligative properties as treated in high school chemistry course. Normally used alcohol or mercury
More informationPhase Transformations in Metals and Alloys
Phase Transformations in Metals and Alloys THIRD EDITION DAVID A. PORTER, KENNETH E. EASTERLING, and MOHAMED Y. SHERIF ( г йс) CRC Press ^ ^ ) Taylor & Francis Group Boca Raton London New York CRC Press
More informationEXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR PRODUCTION ON THE PIERCED FLAT SHEET METAL USING LASER FORMING PROCESS
JOURNAL OF CURRENT RESEARCH IN SCIENCE (ISSN 23225009) CODEN (USA): JCRSDJ 2014, Vol. 2, No. 2, pp:277284 Available at www.jcrs010.com ORIGINAL ARTICLE EXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR
More informationMATERIALS 101 INTRODUCTION TO STRUCTURE AND PROPERTIES WINTER Problem Set 6 Due: Tuesday, March 6, 11:00 AM
Problem Set 6 Due: Tuesday, March 6, 11:00 AM 1. TTT Diagrams Based on the transformation diagrams for eutectoid steel shown below, what microstructure would result from the following cooling histories?
More informationMultiphysics CAE Simulations of Casting Process for the First Time Right Product Development
Multiphysics CAE Simulations of Casting Process for the First Time Right Product Development Mir Mehdi Hussain *, Ramanathan SV, and Raj C Thiagarajan *Corresponding Author ATOA Scientific Technologies
More informationPreparation of Cast Iron Foundry Alloys
Preparation of Cast Iron Foundry Alloys André Luís de Brito Baptísta UFF / EEIMVR  Brazil Cast irons can exhibit a wide range of microstructural constituents depending upon their composition and heat
More informationPreparation Effect of Mould Systems on Microstructure and Mechanical Properties of Spheroidised Graphite Iron
RESEARCH ARTICLE OPEN ACCESS Preparation Effect of Mould Systems on Microstructure and Mechanical Properties of Spheroidised Graphite Iron Ashish Kumar Gupta 1, Dibakor Boruah 2, Nikhil Suresh 3, Nazish
More informationDNVGLCP0249 Edition May 2016
CLASS PROGRAMME Approval of manufacturers DNVGLCP0249 Edition May 2016 The content of this service document is the subject of intellectual property rights reserved by ("DNV GL"). The user accepts that
More informationINDUCTION WELDED SMALL DIAMETER TUBE PRODUCTION LINE
INDUCTION WELDED SMALL DIAMETER TUBE PRODUCTION LINE Target Production of welded single  wall tubing manufactured to ASTM A 513, also zinc coated as per UNI 574166, suitable for many low pressure and
More informationHigh carbon and quenchable steels Hot Rolled Steel Plate and Coil for Hardening and Wear Resistance
Data Sheet: A2.2 High carbon and quenchable steels Hot Rolled Steel Plate and Coil for Hardening and Wear Resistance General description Steel is generally classified as high carbon steel if the nominal
More informationCasting Process Simulation of Compacted Graphite Iron (03025)
Casting Process Simulation of Compacted Graphite Iron (03025) Copyright 2003 American Foundry Society Dipl.Ing. C. Heisser MAGMA Foundry Technologies, Inc., Arlington Heights, Illinois Dr.Ing. Jörg
More informationBINARY SYSTEMS. Definition of Composition: Atomic (molar) fraction. Atomic percent. Mass fraction. Mass percent (weight percent)
BINARY SYSTEMS Definition of Composition: Atomic (molar) fraction Atomic percent Mass fraction Mass percent (weight percent) na =, x i n = A i i i Weight percent mainly in industry! x at % A = x 100 A
More informationDr. Pulak M. Pandey. paniit.iitd.ac.in/ ~ pmpandey
Dr. Pulak M. Pandey http:// paniit.iitd.ac.in/ ~ pmpandey Metals and alloys may not posses all the desired properties in the finished product. Alloying and heat treatment are two methods which are extensively
More informationAblation of Hybrid Metal Matrix Composites
Paper 11057.pdf, Page 1 of 7 Copyright 2011 American Foundry Society Ablation of Hybrid Metal Matrix Composites D. Weiss Eck Industries, Manitowoc, WI J. Grassi Alotech LLC Ltd., Brooklyn, OH B. Schultz,
More informationEFFECT OF In ADDITION ON SnAg SOLDER, ITS WETTING AND SHEAR STRENGTH OF COPPER JOINTS
202 Kovove Mater. 43 2005 202 209 EFFECT OF In ADDITION ON SnAg SOLDER, ITS WETTING AND SHEAR STRENGTH OF COPPER JOINTS PAVOL ŠEBO*, PAVOL ŠTEFÁNIK Institute of Materials and Machine Mechanics, Slovak
More informationInoculation of cast irons: practices and developments
Inoculation of cast irons: practices and developments Dr John Pearce CEng Prof MICME BSc PhD FIM National Metal and Materials, National Science and Tech Development Agency, Ministry of Science and Technology,
More informationThe First Law of Thermodynamics: Closed Systems. Heat Transfer
The First Law of Thermodynamics: Closed Systems The first law of thermodynamics can be simply stated as follows: during an interaction between a system and its surroundings, the amount of energy gained
More informationEffect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel
International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 2832 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia
More informationChapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More informationA NOVEL SINTERINGDISSOLUTION PROCESS FOR MANUFACTURING Al FOAMS
Scripta mater. 44 (2001) 105 110 www.elsevier.com/locate/scriptamat A NOVEL SINTERINGDISSOLUTION PROCESS FOR MANUFACTURING Al FOAMS Y.Y. Zhao and D.X. Sun Materials Science and Engineering, Department
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationEffects of mass transfer processes in designing a heterogeneous catalytic reactor
Project Report 2013 MVK160 Heat and Mass Transport May 13, 2013, Lund, Sweden Effects of mass transfer processes in designing a heterogeneous catalytic reactor Maryneth de Roxas Dept. of Energy Sciences,
More informationDevelopment of a Model for Wet Scrubbing of Carbon Dioxide by Chilled Ammonia
Development of a Model for Wet Scrubbing of Carbon Dioxide by Chilled Ammonia John Nilsson Department of Chemical Engineering, Lund University, P. O. Box 124, SE221 00 Lund, Sweden In this paper, the
More information